Copyright to IJIRSET www.ijirset.com 333
Investigation on Influence of Size of the
Aggregate in Flyash and GGBS Based
Geopolymer Concrete with Complete
Replacement of River Sand by M-Sand
P.Mahalakshmi1, S.Christi2, G.Mahalakshmi3, J.Nithya4
UG Student, Department of Civil Engineering, St.Joseph College of Engineering, India13
Assistant professor, Department of Civil Engineering, St.Joseph College of Engineering, India2
PG Student, Department of Civil Engineering, Gnanamani College of Engineering, Namakkal, India4
ABSTRACT: Concrete is the most commonly used construction material across all over the world. But, due to its increase in productivity, there is a increased emission of CO2 that results in global warming. Hence, there came an existence of newer green material popularly known as “Geopolymer concrete”. In this project work, the influence of size of aggregate content on mechanical properties of Flyash and GGBS based geopolymer concrete were analyzed at low molarity (6M) with complete replacement of river sand by M-Sand. Flyash and GGBS Based geopolymer was tried at low molarity because with increase in molarity of sodium hydroxide solution there is an increase in cost for overall production of geopolymer concrete. At 6M, cost in production of GPC was almost equal to the cost required for the production of normal conventional concrete. All geopolymer concrete mixes were prepared for varying proportion of two different size of aggregate and cured in direct sun light since ground granulated blast furnace slag have a significant effect on the setting time and strength development of Geopolymer concrete. Geopolymer concrete specimens were tested for compressive strength. Testing was done at the ages of 3 days, 7 days and 28 days. Flyash and Ground granulated blast furnace slag based geopolymer concrete give significant strength at 6M molarity of NaOH solution. So ordinary Portland cement concrete can be replaced by ground granulated blast furnace slag based geopolymer concrete which helps in reducing of CO2 during manufacturing of cement by reducing the use of cement
KEYWORDS: flyash, GGBS, M-sand, Geopolymer, ambient curing, compressive strength.
The global use of Ordinary portland cement is second next to water. World business council for sustainable development reveals that 5% of CO2 emission worldwide is from cement industry. This increased level of greenhouse gases which contributes to global warming lead to the necessity to look for a new alternative greener material. In this respect, Geopolymer concrete is one such alternative that shows a promising application in concrete industry. In Geopolymer concrete by-products from different industries such as ground granulated blast furnace slag, Fly Ash and Rice Husk Ash are used as source material, alkaline activator solution combination of alkali hydroxide and alkali silicate is used to activate these source materials so as to form geopolymer mortar which acts as binding material for coarse and fine aggregates to hold them together in the matrix.
Copyright to IJIRSET www.ijirset.com 334 polymeric reaction of alkaline liquid with silicon and aluminium as source material of geological origin or by using byproduct materials such as flyash, GGBS, Rice husk.,etc.’
Flyash, GGBS, alkaline solution and coarse aggregate are the materials used in the preparation of concrete. Flyash is brought from ennore thermal power station which is coal based located in Chennai. GGBS is brought from the local shop available in Chennai. The alkaline solutions used in this study are sodium hydroxide in ﬂake form (NaOH with 98 % purity) dissolved in water and sodium silicate solution (Na2O=14.7%, SiO2 =29.4%, and water=55.9%). Both the solutions are mixed together and the alkaline liquid is prepared at least one day prior to use.
Two types of locally available aggregates comprising 20 mm and 12mm for coarse aggregates and for fine aggregate M-Sand is used.
2.2 Fly ash
Flyash used is an industrial byproduct of coal based thermal power station. In this study, two types of flyash were used, where one was dark grey in colour (20%) and other was light grey (80%) in colour. Dark grey colour flyash imparts good colour to the concrete and also delays the setting time. The properties of fly ash are shown in Table 2.2.
Table 2.2: Properties of fly ash
Figure 2.1 flyash
2.3 Ground Granulated Blast Furnace Slag (GGBS)
Ground granulated blast furnace slag (GGBS) is an industrial by-product resulting from rapid water cooling of molten steel. It is known to have advantageous properties for the concrete industry as it is relatively inexpensive to obtain, highly resistant to chemical attack and maintains excellent thermal properties. Major components of the slag product are SiO2, CaO, MgO and Al2O3. These components are responsible for cementitious property of slag.
S.No Physical properties Result
1. Specific gravity 2.2
2. Physical form Powder
3. Size (Micron) 0.1
4. Colour Dark grey , light grey
Copyright to IJIRSET www.ijirset.com 335 Table 2.2: Properties of fly ash
Figure 2.2 ground granulated blast furnace slag
2.4 Alkaline Activator Solution
In the Geopolymer concrete alkaline activator solution is very important constituents. The most common alkaline activator solution used in geopolymerization is a mixture of Sodium Hydroxide (NaOH) or Potassium Hydroxide (KOH) and Sodium Silicate (Na2SiO3) or Potassium Silicate (K2SiO3). In this experimental work Sodium Hydroxide (NaOH) and Sodium Silicate (Na2SiO3) is used as alkaline activator solution since Al-Si minerals are more soluble in Sodium based compound. Also, the sodium hydroxide solution with a concentration of 6M consisted of 6x40 = 240 grams of sodium hydroxide solids (in flakes form) per litre of the solution, where 40 is the molecular weight of sodium hydroxide is prepared.
Figure 2.3 mixed solution of sodium hydroxide and sodium silicate
S.No Physical properties Result
1. Specific gravity 2.85
2. Physical form Powder
3. Size (Micron) 0.3
4. Colour White
5. Blaine fineness 400 m2 /kg
Copyright to IJIRSET www.ijirset.com 336 2.5 Coarse aggregates
In this study, coarse aggregates of size 12 mm and 20 mm conforming to specifications as given in IS: 383- 1970 is used.
2.6 Fine aggregates
The study is carried by completely replacing river sand with M-Sand so that behaviour of geopolymer concrete with M-Sand is determined. Fine aggregate used in the experimental work have specification conforming to IS: 383- 1970
III. MIX DESIGN 3.1 General
GPC is a new constructional material which has developed in recent decades. So there is no codal provision for mix deign till now. Therefore the methods which has been employed by researchers frequently in past to design the mix have been used in this study. A preliminary study has been carried out to understand basic design method of developing GPC mix. Preliminary study is carried out for 3 days compressive strength of GPC samples to fix certain mixture parameters and to develop an understanding of the trial mix proportioning of GPC. Parameter such as sodium silicate to sodium hydroxide ratio, alkaline solution to binder content ratio, molarity of NaOH and water to geopolymer solids are kept constant and its value are 2.5, 0.4, 6M and 0.25 respectively had taken. Also, the Ratio of flyash and GGBS is taken as 0.7: 0.3.
3.2 Trial 1 mix design:
Unit weight of concrete = 2400 Kg/m3
Total mass of combined aggregates assumed = 78% of 2400 = 1872 Kg/m3
Mass of fine aggregate (Coarse sand) = 38% of 1872 = 711.36 Kg/m3
Mass of coarse aggregates = 1872-711.36 = 1160.64 Kg/m3
Mass of 20 mm coarse aggregates = 52% of 1160.64 = 603.53 Kg/m3
Mass of 12 mm coarse aggregates = 1160.64 – 603.53 = 557.12 Kg/m3
Mass of source material (GGBS) and alkaline liquid = 2400-1872 = 528 Kg/m3
Alkaline liquid to source material ratio = 0.35
Mass of Source material (flyash and GGBS) = 528/ (1.35) = 391.11 Kg/m3
Mass of alkaline liquid = 156.89 Kg/m3
Na2SiO3/NaOH = 2.5
Mass of NaOH solution = 156.89/(1+2.5) = 44.825 kg/m3
Mass of Sodium silicate solution = 156.89-44.825= 112.06 Kg/m3
Problems in trial 1:
Copyright to IJIRSET www.ijirset.com 337 to binder content ratio and molarity of NaOH was very less. To overcome this problem, trial mix 2 is performed with increased alkaline solution to binder content and solution is prepared before 2 hours of casting of the specimen.
3.3 Trial 2 mix design:
In trial 2, all the parameters are as same as that followed in trial mix1, except alkaline to binder content, which is increased to 0.5. Total aggregate content is 75% and that of ratio of fine aggregate to coarse aggregate is 0.35.
Unit weight of concrete = 2400 Kg/m3
Total mass of combined aggregates assumed = 75% of 2400 = 1800 Kg/m3
Mass of fine aggregate (Coarse sand) = 35% of 1800 = 630 Kg/m3
Mass of coarse aggregates = 1800-630 = 1170 Kg/m3
Mass of 20 mm coarse aggregates = 52% of 1170 = 670 Kg/m3
Mass of 12 mm coarse aggregates = 1170– 670 = 500 Kg/m3
Mass of source material (GGBS) and alkaline liquid = 2400-1800= 600 Kg/m3
Alkaline liquid to source material ratio = 0.5
Mass of Source material (flyash and GGBS) = 600/ (1.50) = 400Kg/m3
Mass of alkaline liquid = 200 Kg/m3
Na2SiO3/NaOH = 2.5
Mass of NaOH solution = 200/(1+2.5) = 57.14 kg/m3
Mass of Sodium silicate solution = 200-57.14 = 142.86 Kg/m3
Additional water added = 10% of the binder content = 40 Kg/m3
AVERAGE COMPRESSIVE STRENGTH OF 3 DAY CURING = 22.22 N/mm2
Problems in trial 2:
For trial2, the Surface finish was little good after demoulding of samples. Yet, there was no perfect surface finish and the mix was very stiff. This is due to the large proportion of 20mm aggregate. Thus, to overcome the problem of workability of the concrete and to obtain perfect surface finish, increased proportion of small sized aggregate is taken.
3.4 Mix Proportions
Copyright to IJIRSET www.ijirset.com 338
GGBS = 280 kg/m3
Fly Ash = 120 kg/m3
Water = 120 kg/m3
Sodium hydroxide = 57.14 kg/m3
Sodium silicate solution = 142.86 kg/m3
Fine aggregate = 630 kg/m3
Coarse aggregate = 1170 kg/m3
The table 3.1 shows the mix proportion of concrete.
Table 3.1 Mix proportion
IV. EXPERIMENTAL PROGRAM
4.1 Preparation of alkaline solution
To prepare the alkaline solution of 6M for the manufacture of the geopolymer concrete, 240 grams (6x40) of sodium hydroxide in flakes form is dissolved in one litre of water. This solution is mixed for about 2 minutes until the solids get dissolved in water completely. The required quantity of sodium silicate solution is then mixed with sodium hydroxide. This solution is agitated for about 4 minutes so that proper mixing of the two solutions is ensured. The solution is prepared 2 hours before casting.
Figure 4.1 mixing of solution Mix proportions Flyash kg/m3 GGBS kg/m3 Sodium hydroxide Solution (6M) Sodium silicate solution Fine Aggregate (M-Sand) kg/m3 Coarse Aggregate (20mm) kg/m3 Coarse Aggregate (12mm) kg/m3 Extra Water kg/m3
Mix 1(0%) 120 280 57.14 142.86 630 - 1170 40
Mix 2(20%) 120 280 57.14 142.86 630 234 936 40
Mix 3(40%) 120 280 57.14 142.86 630 468 702 40
Copyright to IJIRSET www.ijirset.com 339 4.2 Casting of the specimen
In this study, hand mixing is adopted. From the table 3.1, the required quantity of aggregate for three cube specimens is taken and spread over the floor for mixing. Since two different size of aggregate (20mm and 12mm) is used, coarse and fine aggregates are mixed together before the addition of the binder. Similarly, flyash and GGBS are mixed together before adding with aggregate. Now the aggregate, binder and alkaline solution are mixed and casted into the cube mould of size 150mm x 150mm x 150mm. Mixing of concrete after the addition of solution is done for about 4 minutes.
Figure 4.3 Adding solutions to the binder and aggregate mixture
4.3 Curing of the specimen
The specimen is demoulded after 24 hours of casting. This specimen is then cured in direct sunlight for 3 day,7 day, 28 day curing.
4.4 Compressive strength Test (Ref: IS: 516-1959)
The compressive strength test was conducted as per IS: 516-1959. The geopolymer concrete specimens were tested for compressive strength after 3, 7 days of direct sun light curing. This test was performed on cube of standard size 150mm×150mm×150mm. the compressive strength of any mix was taken as average of strength of three samples.
All the specimens were tested using a compression testing machine (CTM) of 2000 KN capacity equipped with a monitor to display the results. The failure load and corresponding compressive stress value was read from the screen and noted down. The compressive strength is the ratio of crushing load to the surface area of the specimens expressed in N/mm2.
Copyright to IJIRSET www.ijirset.com 340 V.RESULTS AND DISCUSSION
Compressive strength of the flyash and GGBS based geopolymer was determined by varying the proportion of different size of the aggregate (20mm and 12mm aggregate) at low molarity (6M) and the test results were compared.
5.2 Compressive strength
The compressive strengths were determined for 3 day, 7day and 28 day curing for all the 4 types of mixes.
Table 5.1: Compressive Strength of Cubes with complete replacement of River sand by M- Sand
Curing period (days)
Compressive strength (N/mm2)
Mix 1(0%) Mix 2(20%) Mix 3(40%) Mix 4(60%)
3 days 34.22 30.66 26.66 22.22
7 days 37.77 34.22 29.77 24.44
28 days 38.22 35.11 30.66 25.33
Figure 5.1 Effect of curing period on compressive strength of geopolymer concrete for Mix 1
32 34 36 38 40
3 days 7 days 28 days
Compressive strength (N/mm2)
curing period (days)
Copyright to IJIRSET www.ijirset.com 341 Figure 5.2 Effect of varying proportion of 20mm size aggregate on compressive strength of the geopolymer
Figure 5.3 Comparisons on Influence of 20mm size aggregate on compressive strength of the geopolymer concrete at 3 day, 7 day and 28 day curing
From the figure 5.1, it is found that the compressive strength of the concrete is increased to nearly about 10% from 3 day to 7 day curing and there is no significant increase after 7 day of curing.
The figure 5.2, shows that there is a decrease in compressive strength with increase in proportion of 20mm size aggregate.
Study on the compressive strength of geopolymer concrete made from alkali activated ﬂy ash has been presented. Aggregate of nominal size 20 mm, 12mm and M- sand are used in the study. The alkalis used are Sodium Silicate and Sodium Hydroxide. The curing temperature is carried out at ambient temperature (30 °C). Major conclusions derived based on the present study could be summarized as follows:
0 10 20 30 40
mix 1 mix 2 mix 3 mix 4
Compressive strength (N/mm2)
varying mix proportion
3 day curing
0 10 20 30 40 50
mix 1 mix 2 mix 3 mix 4 Compressive
strength (N/mm2 )
Effect of variation in proportion of 20mm size aggregate on compressive strength of geopolymer concrete
Copyright to IJIRSET www.ijirset.com 342 i. Workability of the concrete decreased with increased proportion of 20mm size aggregate. This indicated that
increased proportion of small sized aggregate increases the workability of the geopolymer concrete.
ii. Production of geopolymer concrete at direct sunlight was made achieved with 70% of GGBS and 30% of flyash. The problem of heat curing is eliminated with addition of GGBS to the concrete.
iii. There is no progressive increase in compressive strength after 3 day and 7 day curing.
iv. Compressive strength of the concrete was increased with decreased proportion of 20mm size aggregate. This proved that, required compressive strength can be achieved with large proportion of small sized aggregate. v. Compressive strength achieved with complete replacement of river sand by M-Sand at 6M molarity was
nominal to be used in the construction industry.
vi. Also proper surface finish is achieved with appropriate selection of total aggregate content, ratio of fine aggregate to total aggregate and size of the aggregate.
1. C. S. Maneesh Kumar, G Manimaran and S Prasanth (May 2015), “An ExperimentalInvestigation on GGBS and fly ash Based geopolymer
Concrete With Replacement of Sand by Quarry Dust” IJERA vol 5, pp 91-95.
2. Davidovits J. (1994), “Properties of Geopolymer Concrete” published in proceedings first International Conferemnce on Alkaline Cements and Concretes, Scientific, Research Institute on Binder and Materials, Kiev state university, Kiev, Ukraine, pp 131-149.
3. Fernandez-Jimenez A., Garcia-Lodeiro, I. and Palomo A. (2007), “Durability of Alkali-Activated Fly Ash Cementitious Materials”, J Mater Sci, 42, pp 3055-3065
4. Benny Joseph and George Mathew ( June 2012), “Influence of aggregate content on the behavior of ﬂy ash based geopolymer concrete”
Scientia Iranica Volume 19, Issue 5, October 2012, Pages 1188-1194
5. Gokhan Gorhan and Gokhan Kurklu (Nov 2013), “The Influence of NaOH Solution on theProperties of Fly Ash Based Geopolymer Mortar
Cured at Different Temperatures” ELSEVIER, Composites: Part B 58, pp 371-377.
6. Hardjito D., Wallah S.E., Sumajouw Dody M.J. and Rangan B.V. (Dec 2014), “Technicalpaper On the Development of Fly Ash Based
Geopolymer Concrete” ACI materials Journal V.101, no. 6, pp 467-472.
7. Rangan B.V. and Lloyd N (June 2010), “Geopolymer Concrete with Fly Ash”, Second International Conference on Sustainable Construction Materials and Technologies, Vol. 3, pp. 1493-1504.
8. Qureshi Mohammed N. and Ghosh S. (May 2014), “Effect of Silicate Content on TheProperties of Alkali Activated Blast Furnace Slag Paste” Arab J Sci Eng 39, pp 5905-5916.
9. Zende Rohit and Mamatha A (July 2015), “Study on Fly Ash and GGBS Based GeopolymerConcrete under Ambient Curing” JETIR vol 2, pp 3082-3087.